Journal of NanomaterialsVolume 2012 (2012), Article ID 875295, 5 pagesdoi:10.1155/2012/875295

Research Article

Facile Fabrication of Sodium Titanate Nanostructures Using Metatitanic Acid () and Its Adsorption Property

Gang Li, Lide Zhang, and Ming Fang

Key Laboratory of Materials Physics, Anhui Key Laboratory of Nanomaterials and Nanostructure, Institute of Solid State Physics, Chinese Academy of Sciences, Hefei 230031, China

Received 13 September 2011; Accepted 13 October 2011

Academic Editor: Chunyi Zhi

Copyright © 2012 Gang Li et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.

Abstract.

Fluffy sodium titanate nanostructures have been fabricated by a simple hydrothermal method with metatitanic acid as precursor. The obtained nanostructures exhibit as the aggregation of nanosheets, and the surface area of the nanostructure is about 110.59 m²/g. Such nanoarchitecture indicates high adsorption capacity to some metal ions, such as Cd²⁺, and the maximum adsorption capacity has been estimated to be 255.18 mg/g. The possible reasons that are responsible after its high adsorption ability, have been ascribed to the tiny structure, the ion-exchange ability and the large surface area of the sodium titanate nanostructures. And this may greatly enlarge its application potential as an adsorbent.

1. Introduction

Environmental problems have been a global tickler that badgers the human’s survival and development [1–5], and various physiochemical methods have been used to remove pollutants from waste water. Nanomaterials have been found to be potential adsorbents that may found great applications in environmental treatment [6–9]. And now there are many kinds of nanostructures that have been fabricated towards high-efficient adsorbents. Materials with enhanced adsorption performance are still challenges.

Sodium titanate is one of the ion exchangers that have been found to have potential application in the treatment of environmental pollutants. In the past decades, many kinds of sodium titanate nanostructures have been fabricated with using various physicochemical methods, including nanotubes, nanowires, nanobelts, and so forth [10–15]. However, as far as we know, many of the fabricated nanostructures have the problem of the cost of the method used. So, it is now a great challenge to fabricate nanostructures with low-cost method. Therefore in this paper, we report fluffy sodium titanate nanostructures which are obtained by a simple hydrothermal method using the low-cost industrial raw materials metatitanic acid (TiO₂ · H₂O) as precursor. And this may greatly enlarge its application potential as an adsorbent.

2. Experimental Details

2.1. Materials

The reagents were of purchased from Shanghai Runjie Chemical Reagent Co., Ltd. All chemicals were analytical grade and used without any further purification.

2.2. Synthesis

In a typical synthesis, 3 g metatitanic acid and 1.6 g NaOH were mixed with 40 mL deionized water under agitation for about 2 h. After that, the mixture was transferred into a teflon-lined stainless steel autoclave and heated in an electric oven at 80°C for 30 h. Then the autoclave was cooled down in the air. Then the white product was harvested by filtration and washed with deionized water for several times until the pH was 12 before drying in air.

2.3. Characterization

The characterization experiments were carried out at room temperature. The phase of the powder was identified by X-ray diffraction (XRD) using a Philips X’Pert Pro MPD with Cu K ( Å) radiation. The morphology, crystalline size, and crystal structure of the sample were determined by Field Emission Scanning Electron Microscopy (FESEM; FEI Sirion-200), transmission electron microscopy (TEM), and high-resolution Transmission Electron Microscopy (HRTEM; JEOL JEM-2010, 200 kV). Thermogravimetric analysis (TGA) measurements were performed on a TGA (Pyris Diamond DSC, PERKIN-ELMER, USA) at a constant heating rate of 10 deg min⁻¹. The porous structure characteristics, including the BET surface area, the pore volume, and the pore size distribution, were obtained from the conventional analysis of nitrogen isotherms measured with specific surface and void ratio analyzer (Omnisorp 100 CX, Coulter, USA). Metal concentrations were measured by Inductively Coupled Plasma Spectrometer (Thermo Scientific iCAP 6000).

2.4. Adsorption Experiments

Adsorption isotherm experiment was performed with various Cd²⁺ concentrations (500, 400, 300, 200, and 100 mg/L, resp.), and the sodium titanate was 1.25 mg/mL at room temperature and 24 h contact. Time-dependent adsorption experiment was performed at the quantity of sodium titanate was 1.25 mg/mL at room temperature, and the Cd²⁺ concentration is 100 mg/L. The concentration of pollutant adsorbed on sodium titanate hierarchical nanostructures, (mol g⁻¹), was calculated from the difference of initial concentration () and final concentration remained in solution after equilibrium (), the volume of the solution () and the mass of sodium titanate hierarchical nanostructures () with the equation .

3. Results and Discussions

The typical XRD pattern of the as-prepared sample is shown in Figure 1(a). The characteristic peak of titanate has been found at around ° accounting for the lamellar ordering of the compound with a high interlamellar distance [16–21]. No other phase, such as TiO₂, is found. Figure 1(b) is the FESEM image of the as-prepared sample. It can be found that there are lots of loose fluffy nanostructures. From further investigation of the TEM image of Figure 2(a), it can be seen that the fluffy nanostructures are constructed by some nanosheets, which is thinner than 10 nm by comparison to the supported carbon film. And the corresponding SAED image indicates its polycrystalline property, which should be mainly ascribed to the too thin layer. EDS spectrum of the fluffy nanostructures is shown in Figure 2(c). Only C, O, Ti, and Na elements are observed. It should be noted that the C element comes from the carbon film of the specimen holder and partially from the carbon spheres. The proximate integer ratio of Na : Ti is around 2 : 3, so the chemical formula of the compound should be Na₂Ti₃O₇.

(a)

(b)

Figure 1: (a) XRD pattern of the as-prepared sample; (b) the FESEM image.

(a)

(b)

(c)

Figure 2: (a) TEM image of the as-prepared sample; (b) the SAED pattern.

The nitrogen ad-desorption isotherms of the sodium titanate nanostructure are investigated in Figure 3(a). The nitrogen ad-desorption isotherms show characteristic type IV isotherm with hysteresis loop, indicating that the sodium titanate nanostructures are composed of connected mesopores. The is evaluated to be 110.59 m²/g. Such porous structure and large BET surface area endow the sodium titanate hierarchical nanostructures with potential application as adsorbent. Figure 3(b) is the TG curve of the sodium titanate nanostructure. The TG measurement was done in the region of 50–700°C at a heating rate of 10°C/min. For the fluffy sodium titanate, the weight loss stopped at around 700°C and the total loss was about 15.5%. The weight loss below 200°C (about 12%) can be ascribed to the removal of surface adsorbed/bound water molecules. As increases the annealing temperature to 700°C (mainly in the range of 200–300°C), the residual weight is 3.5%, which should be ascribed to the loss of water molecules from the interlayer.

(a)

(b)

Figure 3: (a) Nitrogen adsorption-desorption isotherms of the sodium titanate nanostructures; (b) TG curve of the sodium titanate nanostructure.

We chose Cd(II) (heavy metal) to investigate the adsorption performance of the sodium titanate nanostructure. The Cd(II) ion-exchange equilibrium data are graphed in Figure 4(a). Excellent fits of the data were performed with the Langmuir isotherm model expressed as where is the concentration of adsorbed ions in solution at equilibration, is the amount of ions adsorbed to form a monolayer coverage on the adsorbent particle, and is the Langmuir adsorption equilibrium constant. The maximum, Cd(II) adsorption capacities calculated by the adsorption isotherms are 255.18 mg/g (calculated from Langmuir simulation). Figure 4(b) is the time-dependent adsorption behavior investigation of Cd(II) on the sodium titanate nanostructures. The adsorption of the Cd(II) ions on the sodium titanate nanostructure depicts a relative fast adsorption process. About 1 h later, almost 90% Cd(II) ions were removed by the adsorbents, and after 3 h, almost all the Cd(II) were removed. The results of the adsorption of Cd(II) are higher than some previously reported [13]. This should not only be ascribed to the ion-exchange ability of the material. It has been well known that the ability of sodium titanate to eliminate the other metal ions is mainly due to the ion-change ability of the interlayered Na⁺ ions. However, this should also be affected by the diffusion length of the adsorbents. As we all know, the bigger the scale of the adsorbents, the harder the heavy metal ions to exchange with the Na⁺ due to the larger diffusion length from the surface to the inner. So, it can be expected that nanomaterials with very small scale may greatly enhance its adsorption ability via the way to shorten the metal ions diffusion length. Also, it should be noted that as the scale of the adsorbents decreases, the surface area increases greatly. This is also favorable for its adsorption ability.

(a)

(b)

Figure 4: (a) Adsorption isotherm of Cd(II) on the sodium titanate nanostructure. °C, solid line: Langmuir model; (b) time-dependent adsorption curve at pH = 6 and the starting concentration of Cd(II) is 100 mg/L.

4. Conclusion

In conclusion, a fluffy sodium titanate nanostructure was successfully fabricated with utilization of hydrothermal reaction. The fluffy sodium titanate nanostructure exhibits a large surface area of about 110.59 m²/g, and thus it could be expected to have high adsorption capacity to some heavy metal ions (such as Cd(II)). And the maximum adsorption capacity of Cd(II) has been estimated to be 255.18 mg/g. So, this kind of material could be expected to have great potential in the environmental treatment, especially for the elimination of heavy metal ions, such as Cd(II).

Acknowledgments

This work was financially supported by the National Basic Research Program of China (Grant no. 2007CB936601) and National Natural Science Foundation of China (20907055).

References

L. Zhang and M. Fang, “Nanomaterials in pollution trace detection and environmental improvement,” Nano Today, vol. 5, no. 2, pp. 128–142, 2010.

X. Tan, M. Fang, and X. Wang, “Sorption speciation of lanthanides/actinides on minerals by TRLFS, EXAFS and DFT studies: A review,” Molecules, vol. 15, no. 11, pp. 8431–8468, 2010.

P. Liu, W. Cai, M. Fang et al., “Room temperature synthesized rutile TiO₂ nanoparticles induced by laser ablation in liquid and their photocatalytic activity,” Nanotechnology, vol. 20, no. 28, Article ID 285707, 2009.

H. Zeng, W. Cai, P. Liu et al., “ZnO-based hollow nanoparticles by selective etching: Elimination and reconstruction of metal—semiconductor interface, improvement of blue emission and photocatalysis,” ACS Nano, vol. 2, no. 8, pp. 1661–1670, 2008.

P. Liu, W. Cai, Z. Li, H. Zeng, and J. Hu, “Optical study of the reduction of hexavalent chromium by iron-based nanoparticles,” Journal of Nanoscience and Nanotechnology, vol. 10, no. 8, pp. 5389–5392, 2010.

X. Tan, Q. Fan, X. Wang, and B. Grambow, “Eu(III) sorption to TiO₂ (anatase and rutile): batch, XPS, and EXAFS studies,” Environmental Science and Technology, vol. 43, no. 9, pp. 3115–3121, 2009.

X. L. Tan, X. K. Wang, H. Geckeis, and T. H. Rabung, “Sorption of Eu(III) on humic acid or fulvic acid bound to hydrous alumina studied by SEM-EDS, XPS, TRLFS, and batch techniques,” Environmental Science and Technology, vol. 42, no. 17, pp. 6532–6537, 2008.

Q. H. Fan, X. L. Tan, J. X. Li, X. K. Wang, W. S. Wu, and G. Montavon, “Sorption of Eu(III) on attapulgite studied by batch, XPS, and EXAFS techniques,” Environmental Science and Technology, vol. 43, no. 15, pp. 5776–5782, 2009.

X. Tan, M. Fang, C. Chen, S. Yu, and X. Wang, “Counterion effects of nickel and sodium dodecylbenzene sulfonate adsorption to multiwalled carbon nanotubes in aqueous solution,” Carbon, vol. 46, no. 13, pp. 1741–1750, 2008.

X. Song, E. Yang, and Y. Zheng, “Synthesis of Mx Hy Ti₃O₇ nanotubes by simple ion-exchanged process and their adsorption property,” Chinese Science Bulletin, vol. 52, no. 18, pp. 2491–2495, 2007.

L. Xiong, Y. Yang, J. Mai et al., “Adsorption behavior of methylene blue onto titanate nanotubes,” Chemical Engineering Journal, vol. 156, no. 2, pp. 313–320, 2010.

D. Yang, Z. Zheng, Y. Yuan et al., “Sorption induced structural deformation of sodium hexa-titanate nanofibers and their ability to selectively trap radioactive Ra(II) ions from water,” Physical Chemistry Chemical Physics, vol. 12, no. 6, pp. 1271–1277, 2010.

X. Cao, X. Xue, L. Zhu, P. Chen, Y. Song, and M. Chen, “Ultrasensitive Na⁺ exchanging performance of free-standing Fe₃O₄@Na₂Ti₃O₇ nanosheets indicated by fluorescein,” Journal of Materials Chemistry, vol. 20, no. 12, pp. 2322–2328, 2010.

S. S. Liu, C. K. Lee, H. C. Chen, C. C. Wang, and L. C. Juang, “Application of titanate nanotubes for Cu(II) ions adsorptive removal from aqueous solution,” Chemical Engineering Journal, vol. 147, no. 2-3, pp. 188–193, 2009.

M. Liu, L. Piao, S. Ju et al., “Fabrication of micrometer-scale spherical titanate nanotube assemblies with high specific surface area,” Materials Letters, vol. 64, no. 10, pp. 1204–1207, 2010.

C.-K. Lee, S.-S. Liu, and H.-C. Chen, “Application of hydrothermal method derived titanate nanotubes as adsorbents,” Recent Patents on Nanotechnology, vol. 3, no. 3, pp. 203–212, 2009.

R. Ma, Y. Bando, and T. Sasaki, “Nanotubes of lepidocrocite titanates,” Chemical Physics Letters, vol. 380, no. 5-6, pp. 577–582, 2003.

R. Ma, K. Fukuda, T. Sasaki, M. Osada, and Y. Bando, “Structural features of titanate nanotubes/nanobelts revealed by raman, X-ray absorption fine structure and electron diffraction characterizations,” Journal of Physical Chemistry B, vol. 109, no. 13, pp. 6210–6214, 2005.

C. W. Peng, M. Richard-Plouet, T. Y. Ke et al., “Chimie douce route to sodium hydroxo titanate nanowires with modulated structure and conversion to highly photoactive titanium dioxides,” Chemistry of Materials, vol. 20, no. 23, pp. 7228–7236, 2008.

D. Portehault, C. Giordano, C. Sanchez, and M. Antonietti, “Nonaqueous route toward a nanostructured hybrid titanate,” Chemistry of Materials, vol. 22, no. 6, pp. 2125–2131, 2010.

M. Qamar, C. R. Yoon, H. J. Oh et al., “Effect of post treatments on the structure and thermal stability of titanate nanotubes,” Nanotechnology, vol. 17, no. 24, pp. 5922–5929, 2006.